Performance of Low Energy Crumb Rubber Modified Bituminous Mixes
Post on 28-Dec-2016
Embed Size (px)
Procedia - Social and Behavioral Sciences 104 ( 2013 ) 49 58
1877-0428 2013 The Authors. Published by Elsevier Ltd.Selection and peer-review under responsibility of International Scientific Committee.doi: 10.1016/j.sbspro.2013.11.097
2nd Conference of Transportation Research Group of India (2nd CTRG)
Performance of Low Energy Crumb Rubber Modified BituminousMixes
Ambika Behla* , Gajendra Kumara , Girish Sharmaa
a CSIR-Central Road Research Institute, Delhi-Mathura Road, P.O. CRRI, New Delhi-110025, India
Rising energy costs and increased awareness of emission problems in the production of Hot Mix Asphalt (HMA) havebrought attention to the potential benefits of Warm Mix Asphalt (WMA) in India. Warm-mix asphalt is the generic term for a variety of technologies that allow the producers of hot-mix asphalt pavement material to lower the temperatures at which the material is mixed and placed on the road. Crumb Rubber Modified Bitumen (CRMB) is a popular binder in India. CRMB iscomposed of bitumen binder and tyre rubber. Tyre rubber, at various percentages, is added to the binder, addition of tyre rubber into binder results in a new product, which requires higher mixing temperatures compared to the conventional one, aswell as increased mixing time, so as to get the uniformity of the product.
A laboratory study was conducted at CSIR-Central Road Research Institute (CRRI) to investigate, how a commerciallyavailable chemical additive can be used to bring down the mixing and compaction temperature of CRMB mix as compared tothe hot mix CRMB. Four different temperature ranges were considered in this study viz 1000C to 1050C, 1100C to 1150C,1200C to 1250C and 1300C to 1350C to determine the various performance characteristics. The CRMB bituminous mix wasprepared in these four temperature ranges and various mix tests were carried out to indicate to how the lower production and compaction temperatures affect the properties and performance characteristics of the mixes. After the laboratory evaluation it was found that CRMB Warm mix can be successfully produced at temperature as low as 110oC and can be compacted at 80-900C as compared to CRMB hot mix (155oC). Full scale performance study indicate that process is highly energy efficient and environment friendly, warm mixesAfter laboratory evaluation, a test track was successfully laid using low energy Crumb Rubber Modified Bitumen.
2013 The Authors. Published by Elsevier Ltd.
Selection and peer-review under responsibility of International Scientific Committee.
Keywords: Warm Mix Asphalt; Crumb Rubber Modified Bitumen (CRMB); Performance Characteristics
* Corresponding author. Tel.: 09810248680; fax: 011-26845943.E-mail address: email@example.com
Available online at www.sciencedirect.com
2013 The Authors. Published by Elsevier Ltd.Selection and peer-review under responsibility of International Scientific Committee.
50 Ambika Behl et al. / Procedia - Social and Behavioral Sciences 104 ( 2013 ) 49 58
Environmental awareness has been increasing rapidly over the past years. Extensive measures like air pollution reduction targets set by the European Union with the Kyoto protocol have encouraged efforts to reduce pollution. Warm Mix Asphalt (WMA), a new paving technology that originated in Europe, is one of those efforts. It allows a reduction in the temperatures at which asphalt mixes are produced and placed. Its benefits are reduction in energy consumption and reduced emissions from burning fuels, fumes and odours generated at the production plant and the paving site. This paper investigates the potential use of warm mix asphalt to produce Crumb Rubber Modified Bitumen (CRMB) at low temperature to reduce the emissions and to lower the consumption of energy during the production of CRMB bituminous mix.
Bitumen is a useful binder for road construction. The steady increase in high traffic intensity in terms of commercial vehicles, and the significant variation in daily and seasonal temperature demand improved road characteristics. Any improvement in the property of the binder is the need of the hour. The addition of polymers/rubbers typically increases the stiffness of the bitumen and improves its temperature susceptibility. Increased stiffness improves the rutting resistance of the mixture in hot climates and allows the use of relatively softer base bitumen, which in turn, provides better low temperature performance. CRMB is composed of bitumen binder and tyre rubber. Tyre rubber, at various percentages, is added to the binder, addition of tyre rubber into binder results in a new product, which requires higher mixing temperatures compared to the conventional one, as well as increased mixing time, so as to get the uniformity of the product. During construction, the temperature must be high enough to ensure the workability of the mix and yet below the temperature at which excessive binder hardening occur. For little or no improvement in workability, increasing the mix temperature often results in increased plant emissions and fumes at the paving site and binder hardening. All around the globe efforts are being put forward to protect the environment. Currently emphasis is on reducing CO2 emissions in view of reducing greenhouse effect
The objective of this paper is to investigate how a commercially available chemical additive can be used to bring down the mixing and compaction temperature of Crumb Rubber Modified Bituminous mix (CRMB) as compared to the conventional CRMB mix. In addition to indicate to how the lower production and compaction temperatures affect the properties and performance characteristics of the mixes.
2. Laboratory Study 2.1 Material
A paving grade Crumb Rubber Modified Bitumen (CRMB-60) and quartzite aggregates of different sizes (13.2mm, 6mm) and stone dust were obtained from the local quarry and was used in this study.CRMB-60 was manufactured at the plant using 10 to 12% of tyre rubber by weight of bitumen. The tyre rubber used to modify
The modified bitumen was tested for physical properties as per IS73:2006 (test results are given in Table 1) and the physical properties of aggregate were studied to determine its performance as per [IS:2386-1963 (Part 1-6)].The test results are given in Table 2.
51 Ambika Behl et al. / Procedia - Social and Behavioral Sciences 104 ( 2013 ) 49 58
Table 1 Physical Properties of CRMB 60
Sr.No Test Grade & Requirement
Results Obtained Method of Test
1 Penetration at 25oC,0.1mm, 100g, 5sec
52 Ambika Behl et al. / Procedia - Social and Behavioral Sciences 104 ( 2013 ) 49 58
2.3 Mix Design for BC Mix
In this study, design of Bituminous Concrete (BC), grading 2, 30-45mm thick was considered (as per MORTH Specifications for Road and Bridge Works -IV Revision). The Optimum Binder Content (OBC) in hot mix with CRMB-60 was obtained by Marshall bituminous mix design method.
The optimum dose of the additive for the warm bituminous mix determined was 0.5% by weight of the bitumen. The optimum dosage of warm mix additive was determined on the basis of viscosity test. CRMB-60 showed a substantial reduction in viscosity after the addition of 0.2% of the additive and it further reduced to a great extent till 0.5% of addition of the additive. But there was not much reduction observed when the dosage was increased to 0.7% from 0.5%. The optimum reduction in viscosity was observed at the dosage of 0.5% and hence it was selected as the optimum dose of the warm mix additive. The bitumen-aggregate blended with additive was used and Marshall Samples were prepared at different temperature ranges. The various performance tests of the prepared samples were carried out in the laboratory. The behaviour of the warm bituminous mix asphalt was studied and compared with the conventional bituminous mix through various laboratory performance tests for assessing the properties at reduced mixing and compaction temperatures. 2.4 Performance Characteristics of Bituminous Mix
Samples were prepared at OBC and with 0.5% warm mix additive at various temperature ranges and few samples were made (@1550C) without warm mix additive to compare the results of warm mix with conventional hot mix. Four temperature ranges were considered in this study viz 1000C to 1050C, 1100C to 1150C, 1200C to 1250C and 1300C to 1350C to determine the various performance characteristics.
2.4.1 Retained Stability
Retained Stability tests were conducted on Marshall Samples of conventional mix and warm mix. The stability was determined after placing the samples in water bath at 600C for half an hour and 24 hours. The test results are given in table 3.
Table 3 Results of Retained Stability
Type of Mix at Various temperatures Avg. stability after half an hour in water at 600C (kg)
Avg. stability after 24 hours in water at 600C (kg)
Avg. Retained Stability %
CRMB 60 Bitumen @1550C 1600Cwithout additive 1127 885 78.5
Minimum 75% (as per MORTH 4th Revision Table 500-17)
Warm mix additive Modified CRMB @ 1300C- 1350C 1196 999 83.5
Warm mix additive Modified CRMB @ 1200C - 1250C 1156 962 83.2
Warm mix additive Modified CRMB @ 1100C - 1150C 1128 908 80.4
Warm mix additive Modified CRMB @ 1000C - 1050C 1119 895 79.9
53 Ambika Behl et al. / Procedia - Social and Behavioral Sciences 104 ( 2013 ) 49 58
2.4.2 Indirect Tensile Strength (ITS) & Tensile Strength Ratio (TSR)
ITS tests were conducted on Marshall Samples of conventional bituminous mixes and warm mixes at 250C. The ITS test was performed